AG Jotamastic 90 (5) .pdf
Aperçu du document
grease, or fuels, water emulsifiable degreasers-cleaners may be used to remove these contaminants. It is
important to only clean an area that can be fully washed down after degreasing before any of the cleaner can
dry on the surface.
Ultra high pressure water jetting can be used to remove laitance and reveal blowholes and imperfections.
Ensure concrete is dry before coating application.
Dry abrasive blast cleaning to SSPC-SP 13/NACE No. 6. All prepared surfaces should then have all “blow holes”
and other surface defects filled with suitable filler that is compatible with the primer and finish coat system to
ensure that the coating can be applied over a smooth and regular substrate.
Diamond disc grinding
Diamond grind the surface to remove all laitance and expose the aggregates.
Low pressure water washing to a rough, clean, dry and laitance free surface.
Verification of existing coatings including primers
When the surface is an existing coating, verify with technical data sheet and application guide of the involved
products, both over coatability and the given maximum over coating interval.
High pressure water jetting surface preparation refers to ISO 8501-4, for substrates previously coated either
with a full coating system (surface DC A, DC B, DC C) or shop primer (surface DP I and DP Z). The surface
definition for existing coating (DC) refers to the degree of coating breakdown according to ISO 4628.
It is important before considering hydro jetting, to ensure that the specified coating system is compatible with
the existing coating system. High pressure water jetting does not remove mill scale or create surface roughness,
and is only useful for surfaces with an initial roughness suitable for the subsequent coat.
Shop primers are accepted as temporary protection of steel plates and profiles. Refer to the technical data sheet
for the generic types accepted. Certain standards require pre-approval of the shop primer as part of a complete
system. Contact your nearest Jotun office for specific system compatibility. Before being overcoated the shop
primer must be fully cured, clean, dust free, dry and undamaged. Inorganic zinc shop primers must be free of
zinc salts (white rust).
Corroded and damaged areas must be blast cleaned to minimum Sa 1 (ISO 8501-1).
Acceptable environmental conditions - before and during application
Before application, test the atmospheric conditions in the vicinity of the substrate for the dew formation
according to ISO 8502-4.
5 - 60
5 - 60
Relative Humidity (RH)
10 - 85
-5 - 40
Date of issue:
8 February 2017
This Application Guide supersedes those previously issued.
The Application Guide (AG) must be read in conjunction with the relevant specification, Technical Data Sheet (TDS) and Safety
Data Sheet (SDS) for all the products used as part of the coating system.
For your nearest local Jotun office, please visit our website at www.jotun.com.